Toshiro Harada · Hiroshi Matsunaga · Yutaka Kataoka Makoto Kiguchi · Junji Matsumura
Weatherability and combustibility of fi re-retardant-impregnated wood after
accelerated weathering tests
Abstract The weatherability and combustibility of fi re-retardant-impregnated wood during accelerated weather-ing for up to 2000 h were evaluated. The ability of coatweather-ing to retain fi re-retardant chemicals against leaching was also examined using four coating systems (water-borne or solvent-borne, pigmented or clear, fi lm-forming or pene-trating). Furthermore, the distribution of fi re retardants in the specimens was observed by scanning electron micros-copy in combination with energy dispersive analysis of X-rays (SEM-EDX). The fi re performance of the specimens during weathering depended on the chemical retention, and was maintained at a quasi-noncombustible material level if the chemical retention was above 150 kg/m3
. The maximum duration of accelerated weathering to keep this retention was 250 h for the uncoated specimens, but increased to over 1000 h for pigmented coatings. SEM-EDX revealed that the fi re retardants were accumulated in the cell lumina through-out the wood tissues. However, in the uncoated samples, the leaching of fi re retardants occurred for surfaces exposed to light and water, and was observed down to a depth of ∼150 μm after 500 h. The leaching depth extended through-out the specimen after 1000 h. In contrast, the fi re retar-dants still remained in samples fi nished with a solvent-borne pigmented penetrating coating even after 1000 h due to their relatively high chemical retention.
Key words Fire-retardant wood · Cone calorimeter · Accel-erated weathering test · SEM · EDX
T. Harada (*) · H. Matsunaga · Y. Kataoka · M. Kiguchi
Department of Wood Improvement, Forestry and Forest Products Research Institute, 1 Matsunosato, Tsukuba 305-8687, Japan Tel. +81-29-829-8297; Fax +81-29-874-3720
Faculty of Agriculture, Kyushu University, Fukuoka 812-8581, Japan
Part of this article was presented at the 57th Annual Meeting of the Japan Wood Research Society, Hiroshima, Japan, August 2007
The use of wood in exterior applications has increased since 2000, when revisions in the Building Standard Law of Japan started to permit the use of wooden exterior walls if the relevant fi re performance criteria were met. It is well known that the fi re performance of fi re-retardant-treated (FRT) wood depends on the amount of fi re-retardant chemical (FRC) impregnated into the wood. In the case of phospho-rous and nitrogen chemicals, the required amount of chemi-cals is 70–100 kg/m3
to meet the criteria for fi re retardant material and 150–200 kg/m3
for quasi-noncombustible mate-rial, according to the Building Standard Law of Japan.1 However, because the FRC for wood is water soluble, there is a concern that the fi re performance of FRT wood is degraded in exterior applications.
The leaching mechanism of FRC from FRT wood due to weathering has not been fully elucidated, but some impor-tant aspects of the phenomenon are explained as follows. The photodegradation and defi berization of the surface wood cells are induced by exposure to ultraviolet (UV) light. These degradation processes are enhanced by the presence of water. The water absorbed during rainfall penetrates into wood, and this causes slow diffusion of the FRCs toward the surface with resultant loss of the chemi-cals. However, there have been few studies that have reported on the rate of FRC leaching and its infl uence on the fi re performance of FRT wood. There is also still little information on the distribution and diffusion of FRC during weathering and how to prevent it.
The weatherability of FRT wood has already been discussed in Forest Products Laboratory (FPL) reports2–4 and Östman’s reviews.5,6 According to the FPL reports,2,3 which describe natural weathering tests that were conducted for up to 10 years, some of the treatments such as the impregnation of dicyandiamide–phosphoric acid–formalde-hyde showed acceptable performance. Fire tests for roof coverings (Burning brand tests7
) and vertical fl ame spread tests (modifi ed Schlyter tests3
) were also conducted. However, the values for chemical retention after
ing were not shown, and it is not clear whether their results correspond to the fi re performance evaluated by the cone calorimeter test currently being used in Japan.
The average heat release rates for the leached FRT wood were measured by heat release calorimeter,4
but these specimens were leached by placing them in distilled water. More recently, Östman and Tsantaridis6
conducted cone calorimeter tests of FRT wood after leaching by accelerated weathering (ASTM D2898-94)8
and natural weathering, and concluded that the fi re performance of FRT wood could be maintained if the retention levels were high enough. They also reported that paint systems contribute considerably to maintaining the fi re performance of FRT wood in exterior applications. However, these results cannot simply be adopted in Japan because of the differences in the evaluation system of fi re performance between coun-tries. In addition, the distribution of the FRC during weath-ering was not discussed.
In this article, the weatherability of FRT woods was evaluated using a xenon weather meter and their combus-tibility was rated by cone calorimeter test to study quanti-tatively the rate of FRC leaching and the infl uence of FRC loss on the fi re performance. The effect of coating to prevent leaching was also examined using several types of coating systems. Furthermore, the distribution of FRC in the specimens with and without coating was monitored using scanning electron microscopy in combination with energy-dispersive X-ray analysis (SEM-EDX) to examine the leaching mechanism of FRC and the protective effect of coating.
Sugi (Cryptomeria japonica D. Don) sapwood specimens measuring 100 mm (tangential) × 120 mm (longitudinal) × 8 mm (radial) were impregnated with FRC (polyphosphatic carbamate), and were then fi nished with one of four coating systems as will be described. After accelerated weathering
tests, the samples were each cut into two pieces: a large one for the cone calorimeter test, and a smaller one for the observations of FRC distribution and coating systems by SEM-EDX.
The FRC used to treat the wood specimen was the com-mercially available Non-nen OK-201 (Marubishi Oil Chem-ical). The concentration of the undiluted solution was 50%. The main component was polyphosphatic carbamate and the degree of polymerization was 5–10. The chemical com-pound was NH2CO-[OPO(ONH4)]n-OCNH2. The fi re retar-dant was diluted by water to prepare a 25% solution.
The processing procedure was as follows. The specimens were immersed in the fi re-retardant solution and placed in a vacuum at 25 torr (3333 Pa) for 30 min, subjected to pres-surized air [10 kgf/cm2
(0.98 MPa)] for 2 h, and then placed in a vacuum again for 30 min. After impregnation, the spec-imens were removed from the chemical feeder and dried under atmospheric conditions for 1 week and then at 60°C for 10 days until the specimen mass stayed constant. The dry chemical retention was approximately 220 kg/m3
. This amount was calculated from the weight of treating solution that each specimen had absorbed during the treating process and the concentration of the solution.
After the impregnation treatment, the front, back, and lateral surfaces of the specimens were fi nished with one of four coating systems and their end grains were sealed with rubber-based resin. The applied coating systems were (A) water-borne fi lm-forming opaque coating, (B) solvent-borne pigmented penetrating coating, (C) solvent-solvent-borne thin-fi lm-forming pigmented coating, and (D) solvent-borne polyurethane fi re-retardant fi lm-forming clear coating, as shown in Table 1. For comparison, specimens with no impregnation treatment and no coating were also prepared. Five specimens were prepared for each combination of treatment and coating.
Table 1. Overview of coating systems used
Coating system Description Primer Topcoat
Number of layers
Mean coating weighta
Solid content (%)
Number of layers
Mean coating weighta
Solid content (%)
A Water-borne acrylic emulsion paint
Film-forming; opaque; brown 1 84.3 10.3 2 96.7 46.6
166.4 B Solvent-borne alkyd
Penetrating; semitransparent; brown
0 – – 2 118.1 28.9
89.3 C Solvent-borne alkyd
Thin-fi lm-forming; penetrating;
0 – – 2 116.3 32.9
polyurethane clear coating
Film-forming; transparent 1 123.8 25.9 1 103.9 20.0
Accelerated weathering test
The weatherability of specimens was assessed in an acceler-ated weathering chamber (Atras Ci4000) according to JIS K5600-7-7 (xenon lamp method)9
for up to 2000 h. The accelerated weathering regime involved continuous expo-sure to xenon arc UV radiation (0.5 W/m2 at 340 nm = 550 W/m2
for 290–800 nm), and 18 min of deionized water spray every 2 h with a black panel temperature of 65° ± 2°C and a chamber temperature of 40° ± 2°C. Mass loss, reten-tion of chemicals, color change, and water repellency (WR) were evaluated. Specimen mass was measured before and after 250, 500, 750, 1500, and 2000 h of weathering. The retention of chemicals was calculated according to Eq. 1, after the specimens were dried to a constant mass in a dry oven at 60°C. In this study, all of the mass lost during the accelerated weathering test was regarded as the fi re-retardant decrease and the leaching of water-soluble wood extractives was neglected assuming that most of them had been leached out during the fi re-retardant impregnation process.
Rh = R0 − (W0 − Wh)/V (1)
where Rh is the retention of chemicals (kg/m 3
) after h hours of weathering, R0 is the initial retention of chemicals (kg/ m3
), W0 is the initial specimen mass (kg), Wh is the specimen mass (kg) after h hours of weathering, and V is the specimen volume (m3
Color change and water repellent index were measured before and after 500, 1000, 1500, and 2000 h of weathering. A colorimeter (Nihon Denshoku Kogyo NF333) was used to quantify color change at the surface of the specimen as a result of weathering. Color is expressed using the CIE Lab (L*, a*, b*) system. Color change (DE*ab) was calculated according to Eq. 2.
DE*ab = [(DL*)2 + (D
a*)2 + (D b*)2
Water repellency (WR)10
is expressed as a percentage and was determined according to Eq. 3.
WR = [1 − (W2 − W)/(W1 − W)] × 100 (3) where W is the specimen mass before the test, W1 is the specimen mass with approximately 1 g of water dropped with a syringe on the surface, W2 is the specimen mass after the dropped water was wiped off with soft paper 1 min later.
The fi re performance of the specimens was evaluated by a cone calorimeter11
(Toyo Seiki Cone3a). Specimens were prepared with dimensions of 100 mm (tangential) × 100 mm (longitudinal) × 8 mm (radial), and were placed horizon-tally under a cone heater with a heat fl ux of 50 kW/m2
. The heating time was 10 min, the same time used for the quasi-noncombustible material test. A stainless steel cover with an opening of 0.0088 m2
on the upper part was attached. The data were recorded by a computer every 2 s, and the
total heat release for 5 and 10 min (THR5, THR10) was evaluated.
Cone calorimeter tests were conducted for coated speci-mens before and after 500, 1000, 1500, and 2000 h of weath-ering. For the uncoated specimens, the tests were done before and after 250, 500, 1000, and 2000 h of weathering. Specimens with the largest mass loss for the same treatment and weathering condition were selected for the cone calo-rimeter tests.
A sledge microtome was used to reveal the transverse surface of specimens measuring 10 × 10 × 8 mm obtained from unweathered and weathered samples. They were coated with carbon and examined using a scanning electron micro-scope (JEOL JSM-5600LV) equipped with an energy-dis-persive X-ray detector (JEOL JED-2140). This microscope was used to examine and map the distribution of phosphorus in FRT wood samples. The microscope used an accelerating voltage of 15 kV; illuminating current of 1.5 nA; working dis-tance of 20 mm; takeoff and tilt angles of 30° and 0°, respec-tively, and dead and dwell (digital map) times of 15%–20% and 0.2 ms/point, respectively. The elemental peaks detected were P-Ka using a window width of 1.96–2.07 keV. Back-scattered electron images were used in preference to second-ary electron images because they gave better contrast between polyphosphatic carbamate and wood.
Results and discussion
Figure 1 shows the average retentions of FRC for up to 2000 h of accelerated weathering. In the case of specimens without coating, the FRC retention decreased steeply from the beginning. The initial chemical retention of 220 kg/m3 decreased to 76 kg/m3 at 500 h, 27 kg/m3 at 1000 h, and 11 kg/m3
at 2000 h. On the other hand, specimens with coat-ings had chemical retention of 175–191 kg/m3
after 750 h of weathering. However, differences could be seen in leach resistance at 1000 h and later depending on the type of coating. The chemical retention of type B was 150 kg/m3
, whereas that of types A and C was 80 kg/m3
and that of type D decreased to the same level of retention as the uncoated specimens (13 kg/m3) after 2000 h of weathering.
The higher retention values for the coated specimens compared with the uncoated specimens indicate that the leaching of FRC can be reduced to a considerable extent by coating. Our results are in accordance with those of Östman and Tsantaridis6
who suggested the protective effect of coating in preventing FRC leaching.
The difference in coating weight is also considered to be a contributing factor. Mean dry coating weights of coating systems A, B, C, and D were calculated to be 123, 60, 69, and 21 g/m2
, respectively, based on their wet weights and solid contents in Table 1. Lower coating weight may be one reason for more leaching but it is generally known that the weatherability of clear coating is inferior to pigmented coating. In this study, the performance of coatings after accelerated weathering tests as mentioned later supported this notion and it is considered that clear coating D allowed UV penetration more easily and deterioration of the wood– coating interface occurred more quickly than with the pig-mented coatings.
It was interesting that among the pigmented coatings used here, the penetrating type B showed better retention values than the fi lm-forming types A and C. As discussed below, SEM observation revealed that coating B penetrated into wood surface cells to generate a protective zone beneath the surface, instead of forming a fi lm on it. The difference in the protection mechanism between the coatings of the highest and the lowest retentions is discussed below in terms of results from SEM-EDX analysis.
Performance of coatings on FRT wood
It is important to evaluate the performance of coating systems on FRT wood because FRC in wood may nega-tively affect it. Thus, changes in WR and changes in color were monitored during accelerated weathering, as shown in Figs. 2 and 3, respectively.
It can be seen in Fig. 2 that the specimens with the pig-mented coatings A, B, and C showed much smaller changes in WR than specimens coated with the clear coating D, which started to decrease in WR after 500 h and dropped to almost the same level as for the uncoated specimens at 1000 h. This result agrees with the results for FRC reten-0
50 100 150 200 250
Test time of accelerated weathering (hr)
ons of fi
500 1000 1500 2000 2500
Fig. 1. Retentions of fi re-retardant chemicals for up to 2000 h of
ac-celerated weathering. Diamonds, water-borne fi lm-forming opaque coating A (see Table 1); squares, solvent-borne pigmented penetrating coating B; triangles, solvent-borne thin-fi lm-forming pigmented coating C; circles, solvent-borne polyurethane fi re-retardant fi lm-forming clear coating D; stars, no coating
0 20 40 60 80 100 120
Test time of accelerated weathering (hr)
Water repellency on surface (%)
0 500 1000 1500 2000 2500
Fig. 2. Water repellency on surface for up to 2000 h of accelerated
weathering. Diamonds, coating A; squares, coating B; triangles, coating C; circles, coating D; stars, no coating; fi lled symbols, fi re-retardant-impregnated samples; open symbols, fi re-retardant-free samples
0 5 10 15 20 25 30
Test time of accelerated weathering (hr)
0 500 1000 1500 2000 2500
Fig. 3. Color change on surface for up to 2000 h of accelerated
tion, which also demonstrated that the protective effect of coating was enhanced by the presence of pigments.
However, it appeared that such effects of coatings could be degraded by the presence of FRC in wood. Figure 2 shows that WR of the coated specimens was slightly lower for the FRT wood than for FRC-free wood. This tendency was most obvious for the specimens treated with coating D, suggesting that the negative impact of FRC on the coating performance may have become more signifi cant for the coatings with relatively low performance.
Figure 3 shows color differences (DE*ab) on the surface during the accelerated weathering. The pigmented coatings A, B, and C tended to show smaller DE*ab than the clear coating D, particularly for the specimens treated with coating A, which showed DE*ab values of less than 6 through-out the weathering test. However, DE*ab for specimens treated with coating C became as large as the value for specimens treated with coating D with increasing weather-ing time. These results are in accordance with those men-tioned above, which suggested that pigments were effective in preventing degradation.
On the other hand, it was not clear whether the presence of FRC enhanced the color change, but the large difference observed at 500 h between samples with and without FRC for specimens treated with coating D may suggest it. Thus, attention should be paid to such negative effects of FRC on the coating performance, although this depends on both the type of FRC and the coating system.
Figure 4 illustrates the relationships between THR10 and the duration of accelerated weathering. THR10 of fi
re-retardant-free specimen varied from 42 to 54 MJ/m2 and this depended on the mass difference between wood speci-mens rather than the effect of coatings. THR10 of FRT woods before weathering was less than 8 MJ/m2
, which is the value required for quasi-noncombustible materials in the Building Standard Law of Japan.
For specimens treated with coating D and those without coating, THR10 exceeded 8 MJ/m2
at 500 h and went up to 14–17 MJ/m2
at 1000 h and 27–29 MJ/m2
at 2000 h, respec-tively. Their chemical retention was 11–13 kg/m3
, which is 5% of the initial retention. However, the THR10 values were 60% of the FRC-free wood specimen, and it is said that a low retention of FRC may have a certain degree of effect on fi re performance.
THR10 of specimens coated with A, B, or C was less than 8 MJ/m2
for up to 1000 h. For up to 2000 h, THR10 was 7.4 MJ/m2
for specimens coated with B and 17–19 MJ/m2 for specimens coated with A or C.
Figure 5 shows the relationships between the retentions of FRC in wood and their fi re performance. As a previous study1
reported, THR10 correlated with the retention of FRC in wood. However, after accelerated weathering tests, THR10 of specimens treated with coating D was higher than other coated specimens with the same amount of chemical retention. Coating system D deteriorated more quickly than the others and fi re-retardant chemicals were partially leached out through checking as observed in SEM-EDX analysis. Therefore, THR10 of specimens treated with coating D was high for its chemical retention. In this study, the fi re performance of FRT wood could be maintained at a quasi-noncombustible material level if WR was main-tained near 100% and the retention of FRC was kept at more than 150 kg/m3
even after leaching. Without coating, more than 60 kg/m3
of FRC was retained at 500 h, THR10
0 10 20 30 40 50 60
Test time of accelerated weathering (hr)
ease for 10 mi
0 500 1000 1500 2000 2500
Fig. 4. Total heat release for 10-min cone calorimeter tests for up to
2000 h of accelerated weathering. Cross, fi re-retardant-free sample with no coating; other symbols correspond to those used in Fig. 2
0 10 20 30 40 50 60
0 50 100 150 200 250
Retention of fire-retardant chemicals (kg/m )3
ease for 10 mi
Fig. 5. Relationships between fi re-retardant chemical retention and
was 9.3 MJ/m2
, but THR5 was 4.2 MJ/m2
and the fi re perfor-mance was equivalent to the fi re-retardant material level.
There were no clear correlations between fi re perfor-mance, WR, and color change. However, WR can become one of the evaluation indices used for maintaining fi re-retardant-impregnated and surface-coated wood, because decreases in WR refl ect the deterioration of the wood– coating interface that accelerates the leaching of FRC.
FRC distribution and protective effect of coating system
Figures 6–11 show scanning backscattered electron and EDX mapping images from sections of the unweathered and weathered FRT wood specimens with and without coating. Numerous white deposits can be clearly seen in unweathered specimens with no coating (Fig. 6A). These deposits are accumulated in the lumina of tracheids. EDX
Fig. 6A, B. Scanning electron
microscopy-energy dispersive X-ray analysis (SEM-EDX) color mapping of a cross section of fi re-retardant-treated (FRT) sugi sapwood uncoated and unweathered: A backscattered electron image; B P-Ka X-ray image. The warmth of colors in the map represents the intensity of X-rays, with white indicating a high intensity, and therefore a high concentration of
Fig. 7A, B. SEM-EDX color
mapping of a cross section of FRT sugi sapwood uncoated and exposed to 500 h of accelerated weathering: A backscattered electron image; B P-Ka X-ray image. Arrows mark erosion
Fig. 8A, B. SEM-EDX color
mapping of a cross section of FRT sugi sapwood uncoated and exposed to 1000 h of accelerated weathering:
Fig. 9A, B. SEM-EDX color
mapping of a cross section of FRT sugi sapwood treated with coating D and exposed to 500 h of accelerated weathering:
A backscattered electron image; B P-Ka X-ray image. Arrows mark checking
Fig. 10A, B. SEM-EDX color
mapping of a cross section of FRT sugi sapwood treated with coating D and exposed to 1000 h of accelerated weathering:
A backscattered electron image; B P-Ka X-ray image. Circled areas show where the fi re-retardant chemical leached out from the checking
Fig. 11A, B. SEM-EDX color
mapping of a cross section of FRT sugi sapwood treated with coating B and exposed to 1000 h of accelerated weathering:
A backscattered electron image; B P-Ka X-ray image. Arrowed areas show where coating B remains in the surface tracheids
mapping confi rmed that the deposits contained phosphorus (Fig. 6B). The uncoated samples exposed to accelerated weathering for 500 h underwent surface erosion (Fig. 7A). Leaching of phosphorus deposits from the lumina of tra-cheids was also observed down to a depth of ∼150 μm from the surface. The leaching depth was then broadly extended
throughout the specimen after 1000 h of accelerated weath-ering (Fig. 8).
study was also easily leached out (Figs. 7, 8) by accelerated weathering.
The effect of coating to prevent the leaching of FRC was examined by comparing coatings D and B, which show the lowest and the highest retention values in Fig. 1, respec-tively. Figure 9 represents an FRT wood specimen coated with the clear, fi lm-forming coating D and exposed to accel-erated weathering for 500 h. A coating layer remained on the surface, but checking could be seen (Fig. 9A), which may explain why the deposits were still present in the lumina of tracheids (Fig. 9B).
The 1000-h exposure to accelerated weathering, however, made the clear coating D exfoliate and caused surface erosion. The FRC was leached out from the weathered surface, especially through checks developed from the surface (Fig. 10). As mentioned earlier, the protective effect of clear coating D may have decreased more rapidly com-pared with the pigmented coatings due to UV degradation of the wood–coating interface.
In contrast, the pigmented, penetrating coating B had the greatest ability to keep the FRC within the wood (Fig. 11). In Fig. 11, it can be seen that coating B penetrated into the tracheid lumina beneath the surface. This protective zone still remained even after 1000 h of accelerated weath-ering (Fig. 11A). This may explain why the FRC deposits were also present at 1000 h (Fig. 11B).
The distribution of the FRC was similar to that of the unweathered control (Fig. 6). The results may account for why the total heat release of this sample was as low as the control sample (0 h, no coating).
The fi re performance of FRT wood during accelerated weathering depended on the retention of FRC against leaching. Pigmented coatings for surface protection showed better retentions than the clear coating, presumably because of their ability to decrease UV penetration into the wood– coating interface. The best retention achieved by pigmented and penetrating coatings shows the possibility of keeping the fi re performance required for quasi-noncombustible material, even after 2000 h of accelerated weathering. SEM-EDX revealed that leaching of FRC occurred on uncoated surfaces to a depth of ∼150 μm after 500 h and extended throughout the specimen after 1000 h. In contrast, leaching was not signifi cant for coated surfaces if the coating sub-stances remained as a barrier. These results indicate that
the proper combination of FRC and coating may enable FRT wood to be used in exterior applications. Further research will compare the fi re performance of FRT woods exposed to natural and artifi cial weathering.
Acknowledgments The authors are very grateful for the fi nancial
support for this research provided by Ministry of Education, Culture, Sports, Science, and Technology of Japan (Grant-in-Aid for Scientifi c Research no. 18580169).
1. Harada T, Uesugi S, Taniuchi H (2003) Evaluation of fi re-retardant wood treated with poly-phosphatic carbamate using a cone calorimeter. Forest Prod J 53:81–85
2. Holmes CA, Knispel RO (1981) Exterior weathering durability of some leach-resistant fi re-retardant treatments for wood shingles: a fi ve-year report. Research Paper FPL403, United States Depart-ment of Agriculture, Forest Products Laboratory, Madison, WI 3. LeVan SL, Holmes CA (1986) Effectiveness of fi re-retardant
treat-ments for shingles after 10 years of outdoor weathering. Research Paper FPL474, United States Department of Agriculture, Forest Products Laboratory, Madison, WI
4. Sweet MS, LeVan SL, White RH, Tran HC, De Groot R (1996) Fire performance of wood treated with combined fi re-retardant and preservative system. Research Paper FPL-RP-545, United States Department of Agriculture, Forest Products Laboratory, Madison, WI
5. Östman B, Angelika V, Hughes A, Hovde PJ, Grexa O (2001) Durability of fi re retardant treated wood products at humid and exterior conditions. Review of literature. Fire Mater 25:95–104 6. Östman BA, Tsantaridis LD (2007) Durability of the reaction to
fi re performance of FRT wood products in interior and exterior applications. Proceedings of InterFlam2007 11th International Fire Science and Engineering Conference, 3–5 September, London, vol 1, pp 33–44
7. American Society for Testing and Materials (2004) ASTM Fire Standards 6th edn. ASTM E 108-04 Standard test methods for fi re tests of roof coverings. ASTM International, West Conshohocken, pp 1019–1027
8. American Society for Testing and Materials (2004) ASTM Fire Standards 6th edn. ASTM D 2898-94 Standard test methods for accelerated weathering of fi re-retardant-treated wood for fi re testing. ASTM International, West Conshohocken, pp 476–477 9. Japanese Standards Association (2008) JIS K5600-7-7. Testing
methods for paints. Part 7: long-period performance of fi lm. Section 7: accelerated weathering and exposure to artifi cial radiation (exposure to fi ltered xenon-arc radiation). Japanese Standards Association, Tokyo
10. Kiguchi M, Kataoka Y, Suzuki M, Imamura Y (2005) Progress towards the service life prediction of coatings for exterior wood by weathering test trials. In: Martin JW, Ryntz RA, Dickie RA (eds) Service life prediction – challenging the status quo. Federation of Societies for Coating Technology, Philadelphia, PA, pp 123–134 11. International Organization for Standardization (2002)